Alloying Effect on Hot Workability of M42 High Speed Steel
In the present study, the effect of Si, Al, Ti, Zr, and Nb addition on the microstructure and hot workability of cast M42 tool steels, basically consisting of 1.0C, 0.2Mn, 3.8Cr, 1.5W, 8.5Co, 9.2Mo, and 1.0V in weight percent has been investigated. Tool steels containing Si of 0.25 and 0.5wt.%, Al of 0.06 and 0.12wt.%, Ti of 0.3wt.%, Zr of 0.3wt.%, and Nb of 0.3wt.% were cast into ingots of 140mm ´ 140mm ´ 330mm by vacuum induction melting. After solution treatment at 1150oC for 1.5hr followed by furnace cooling, hot rolling at 1180oC was conducted on the ingots. Addition of titanium, zirconium and niobium was found to retard the decomposition of the eutectic carbides and result in the deterioration of hot workability of the tool steels, while addition of aluminum and silicon showed relatively well decomposed carbide structure and resulted in sound hot rolled plates.
Digital Object Identifier (DOI): doi.org/10.5281/zenodo.1091640Procedia APA BibTeX Chicago EndNote Harvard JSON MLA RIS XML ISO 690 PDF Downloads 2222
 G. Robert, G. Krauss, and R. Kennedy, Tool steels, 5thedn., ASM International, Materials Park, OH,1998.
 G. Hoyle,High speed tool steels, Butterworth, Cambridge,1988.
 J. R. Davis, Tool materials, ASM International, Materials Park, OH,1995.
 W. Crafts and J. L. Lamont, Trans. A.I.M.E, vol. 180,p. 471,1949.
 H. Fredricksson, M. Hillert, and M. Nica,Scand. J. Metall., vol. 8, p. 115, 1979.
 H. Di, Z. Zhang, G. Wang, and Z. Liu, J. Mater. Proc. Tech., vol. 166, p.359, 2005.
 M. Boccalini, and H. Goldenstein, Inter. Mater. Rev., vol. 46, p. 92, 2001.
 H. Brandis, T.E.T.B., vol. 3, p. 81, 1981.
 C. A. C. Imbert, and H. J. McQueen, Mater. Sci. Eng., vol. A313, p. 104, 2001.
 Y. Li, Q. Jiang, Y. Zhao, and Z. He, J. Mater. Sci. Tech., vol. 13, p.471, 1997.